#------------------------------------------------------------------------------
#$Date: 2016-03-24 14:36:54 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179669 $
#$URL: svn://www.crystallography.net/cod/cif/4/51/22/4512293.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4512293
loop_
_publ_author_name
'Zhao, Jun-Wei'
'Cao, Jing'
'Li, Yan-Zhou'
'Zhang, Jing'
'Chen, Li-Juan'
_publ_section_title
;
 First Tungstoantimonate-Based Transition-Metal--Lanthanide Heterometallic
 Hybrids Functionalized by Amino Acid Ligands
;
_journal_issue                   12
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              6217
_journal_paper_doi               10.1021/cg5007988
_journal_volume                  14
_journal_year                    2014
_chemical_formula_sum            'C8 H110 Fe4 N2 Nd2 O118 Sb2 W18'
_chemical_formula_weight         6187.66
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                107.0660(10)
_cell_angle_beta                 100.0030(10)
_cell_angle_gamma                96.7300(10)
_cell_formula_units_Z            1
_cell_length_a                   12.6125(6)
_cell_length_b                   13.5912(7)
_cell_length_c                   16.2958(8)
_cell_measurement_reflns_used    8956
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      1.72
_cell_volume                     2587.5(2)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean none
_diffrn_measured_fraction_theta_full 0.983
_diffrn_measured_fraction_theta_max 0.983
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0367
_diffrn_reflns_av_sigmaI/netI    0.0681
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            13006
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.72
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    22.084
_exptl_absorpt_correction_T_max  0.2412
_exptl_absorpt_correction_T_min  0.0320
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'green yellow'
_exptl_crystal_density_diffrn    3.971
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'cubic block'
_exptl_crystal_F_000             2774
_exptl_crystal_size_max          0.50
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.09
_refine_diff_density_max         5.648
_refine_diff_density_min         -6.355
_refine_diff_density_rms         0.809
_refine_ls_extinction_coef       0.00042(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     644
_refine_ls_number_reflns         8956
_refine_ls_number_restraints     127
_refine_ls_restrained_S_all      1.033
_refine_ls_R_factor_all          0.0845
_refine_ls_R_factor_gt           0.0795
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1631P)²+135.1124P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2215
_refine_ls_wR_factor_ref         0.2269
_reflns_number_gt                8090
_reflns_number_total             8956
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg5007988_si_002.cif
_cod_data_source_block           2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4512292--4512298.cif.
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4512293
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sb1 Sb 0.35733(10) 0.36009(10) 0.34621(9) 0.0089(3) Uani 1 1 d .
W1 W 0.35688(7) 0.61540(6) 0.47128(6) 0.0121(2) Uani 1 1 d .
W2 W 0.09822(7) 0.48722(7) 0.37952(6) 0.0146(3) Uani 1 1 d .
W3 W 0.24889(7) 0.57396(7) 0.25644(6) 0.0153(3) Uani 1 1 d .
W4 W 0.46895(7) 0.43840(7) 0.18033(6) 0.0135(2) Uani 1 1 d .
W5 W 0.21522(7) 0.31113(7) 0.09685(6) 0.0139(2) Uani 1 1 d .
W6 W 0.04605(7) 0.21569(7) 0.23249(6) 0.0133(2) Uani 1 1 d .
W7 W 0.15209(7) 0.25571(7) 0.44319(6) 0.0145(3) Uani 1 1 d .
W8 W 0.24688(7) 0.09057(7) 0.29042(6) 0.0149(3) Uani 1 1 d .
W9 W 0.41500(7) 0.18406(7) 0.15411(6) 0.0159(3) Uani 1 1 d .
Fe1 Fe 0.3801(2) 0.4307(2) 0.6000(2) 0.0130(6) Uani 1 1 d .
O1W O 0.2404(12) 0.4521(13) 0.6523(11) 0.021(3) Uani 1 1 d U
O2W O 0.4095(17) 0.3192(15) 0.6627(15) 0.039(5) Uani 1 1 d .
O5W O 0.049(3) 0.405(3) -0.118(2) 0.082 Uiso 1 1 d .
O6W O 0.279(2) 0.376(2) -0.0961(14) 0.064(8) Uani 1 1 d .
O7W O 0.078(4) 0.340(3) -0.271(3) 0.118(14) Uiso 1 1 d .
O8W O -0.063(3) 0.182(3) -0.282(2) 0.084 Uiso 1 1 d .
O9W O 0.243(3) 0.222(3) -0.270(2) 0.093(11) Uani 1 1 d .
O10W O 0.079(4) 0.055(4) -0.282(3) 0.121(14) Uiso 1 1 d .
O11W O 0.019(3) 0.103(3) -0.124(3) 0.097(11) Uani 1 1 d U
O12W O 0.259(3) 0.143(2) -0.122(2) 0.083(10) Uani 1 1 d .
O13W O 0.209(10) 0.015(5) 0.583(5) 0.15(4) Uani 0.50 1 d P
O14W O 0.356(4) 0.883(3) 0.402(2) 0.108(14) Uani 1 1 d .
O15W O -0.086(6) 0.461(5) -0.007(5) 0.10(2) Uani 0.50 1 d P
O16W O -0.132(2) 0.199(3) -0.0098(18) 0.079(9) Uani 1 1 d .
O17W O 0.115(3) -0.004(3) 0.002(2) 0.093(11) Uani 1 1 d .
O18W O -0.096(3) 0.394(2) 0.1275(17) 0.070(8) Uani 1 1 d .
O19W O 0.254(3) 0.644(2) 0.768(2) 0.085(11) Uani 1 1 d .
O20W O -0.118(3) 0.203(3) 0.554(3) 0.103(12) Uani 1 1 d .
O21W O 0.1664(16) 0.7125(17) 0.6321(15) 0.043(5) Uani 1 1 d .
O23W O 0.303(4) 0.950(4) 0.861(4) 0.140(17) Uiso 1 1 d .
O22W O 0.675(8) 0.114(8) 0.095(7) 0.13(3) Uiso 0.50 1 d P
O24W O 0.391(4) 1.048(4) 0.825(3) 0.051(11) Uani 0.50 1 d PU
O25W O 0.376(3) 0.133(2) 0.5432(17) 0.079(10) Uani 1 1 d .
O1 O 0.4831(13) 0.5907(13) 0.4398(13) 0.028(4) Uani 1 1 d .
O2 O 0.2751(12) 0.4774(11) 0.3542(9) 0.012(3) Uani 1 1 d U
O3 O 0.3546(13) 0.5299(12) 0.5347(11) 0.022(4) Uani 1 1 d .
O4 O 0.3942(14) 0.7430(13) 0.5502(11) 0.023(4) Uani 1 1 d .
O5 O 0.3169(14) 0.6712(13) 0.3679(12) 0.008(3) Uani 0.80 1 d PU
O5' O 0.352(6) 0.626(5) 0.335(5) 0.010 Uiso 0.20 1 d P
O6 O 0.1935(14) 0.6045(15) 0.4654(12) 0.011 Uiso 0.80 1 d P
O6' O 0.207(6) 0.550(6) 0.467(5) 0.010 Uiso 0.20 1 d P
O7 O -0.0252(13) 0.5192(13) 0.3965(11) 0.021(4) Uani 1 1 d .
O8 O 0.1251(12) 0.3965(11) 0.4462(10) 0.013(3) Uani 1 1 d U
O9 O 0.0492(11) 0.3610(11) 0.2750(9) 0.012(3) Uani 1 1 d .
O10 O 0.1129(14) 0.5590(14) 0.2947(12) 0.010 Uiso 0.80 1 d P
O10' O 0.097(6) 0.497(6) 0.261(5) 0.010 Uiso 0.20 1 d P
O11 O 0.2240(13) 0.6605(14) 0.1993(12) 0.023(4) Uani 1 1 d .
O12 O 0.1854(11) 0.4353(11) 0.1669(9) 0.010(3) Uani 1 1 d U
O13 O 0.3875(12) 0.5465(12) 0.2342(10) 0.016(3) Uiso 1 1 d .
O14 O 0.3469(11) 0.3317(11) 0.2197(10) 0.011(3) Uani 1 1 d U
O15 O 0.5573(13) 0.5106(13) 0.1405(12) 0.025(4) Uani 1 1 d .
O16 O 0.5016(12) 0.3008(11) 0.1347(10) 0.013(3) Uani 1 1 d U
O17 O 0.5427(13) 0.4578(11) 0.2900(11) 0.017(3) Uani 1 1 d U
O18 O 0.3398(12) 0.3929(12) 0.0808(10) 0.017(3) Uani 1 1 d U
O19 O 0.1370(14) 0.2927(12) -0.0037(12) 0.024(4) Uani 1 1 d .
O20 O 0.2912(13) 0.1941(12) 0.0686(11) 0.019(3) Uani 1 1 d U
O21 O 0.1190(12) 0.2356(11) 0.1428(10) 0.015(3) Uani 1 1 d .
O22 O -0.0854(13) 0.1709(13) 0.1697(10) 0.020(3) Uani 1 1 d U
O23 O 0.2204(11) 0.2556(11) 0.3200(9) 0.012(3) Uani 1 1 d U
O24 O 0.0970(12) 0.0849(11) 0.2198(11) 0.016(3) Uani 1 1 d .
O25 O 0.0231(12) 0.2146(12) 0.3441(10) 0.016(3) Uani 1 1 d U
O26 O 0.0873(14) 0.2389(14) 0.5224(12) 0.029(4) Uani 1 1 d .
O27 O 0.1836(12) 0.1188(11) 0.3958(10) 0.015(3) Uani 1 1 d U
O28 O 0.2926(12) 0.3155(11) 0.5009(10) 0.012(3) Uani 1 1 d U
O29 O 0.2370(13) -0.0433(12) 0.2685(11) 0.020(3) Uani 1 1 d U
O30 O 0.3019(12) 0.1096(12) 0.1926(10) 0.017(3) Uani 1 1 d .
O31 O 0.3829(14) 0.1426(13) 0.3635(11) 0.024(4) Uani 1 1 d .
O32 O 0.4567(13) 0.0806(13) 0.0855(12) 0.024(4) Uani 1 1 d .
O33 O 0.5044(13) 0.2059(12) 0.2596(12) 0.022(4) Uani 1 1 d U
Nd1 Nd 0.11627(12) 0.23495(11) -0.17097(9) 0.0276(4) Uani 1 1 d .
Fe2 Fe 0.5328(3) 0.1346(2) 0.3463(2) 0.0176(7) Uani 1 1 d .
O3W O 0.6892(15) 0.1214(16) 0.3258(14) 0.038(5) Uani 1 1 d U
O4W O 0.5497(18) 0.0435(16) 0.4268(16) 0.044(5) Uani 1 1 d .
O34 O 0.4803(15) -0.0061(13) 0.2500(12) 0.027(4) Uani 1 1 d .
O35 O 0.568(3) -0.129(3) 0.258(2) 0.088 Uiso 1 1 d .
H35A H 0.5881 -0.0989 0.3115 0.131 Uiso 1 1 calc R
O36 O 0.520(3) -0.210(3) 0.048(2) 0.083 Uiso 1 1 d .
H36A H 0.5573 -0.1535 0.0788 0.125 Uiso 1 1 calc R
N1 N 0.337(4) -0.118(4) 0.105(3) 0.103(14) Uiso 1 1 d D
H1A H 0.3334 -0.1275 0.0495 0.123 Uiso 1 1 calc R
H1B H 0.3034 -0.0732 0.1337 0.123 Uiso 1 1 calc R
C1 C 0.496(4) -0.088(4) 0.228(4) 0.081 Uiso 1 1 d .
C2 C 0.403(4) -0.178(4) 0.149(3) 0.082 Uiso 1 1 d D
H2A H 0.3549 -0.2138 0.1775 0.098 Uiso 1 1 calc R
C3 C 0.461(4) -0.255(3) 0.102(3) 0.069(12) Uani 1 1 d .
H3A H 0.5103 -0.2793 0.1420 0.083 Uiso 1 1 calc R
C4 C 0.366(5) -0.355(4) 0.028(4) 0.093(16) Uani 1 1 d U
H4A H 0.4029 -0.4072 -0.0036 0.140 Uiso 1 1 calc R
H4D H 0.3220 -0.3297 -0.0119 0.140 Uiso 1 1 calc R
H4B H 0.3211 -0.3862 0.0592 0.140 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O14 Sb1 O2 92.4(6) . .
O14 Sb1 O23 89.7(6) . .
O2 Sb1 O23 92.3(6) . .
O3 W1 O4 104.6(8) . .
O3 W1 O1 96.0(8) . .
O4 W1 O1 103.1(8) . .
O3 W1 O6' 67(2) . .
O4 W1 O6' 111(2) . .
O1 W1 O6' 144(2) . .
O3 W1 O6 86.3(7) . .
O4 W1 O6 95.6(8) . .
O1 W1 O6 159.9(8) . .
O6' W1 O6 23(2) . .
O3 W1 O5 159.4(7) . .
O4 W1 O5 93.3(7) . .
O1 W1 O5 89.7(8) . .
O6' W1 O5 97(2) . .
O6 W1 O5 81.8(7) . .
O3 W1 O2 87.3(7) . .
O4 W1 O2 163.6(6) . .
O1 W1 O2 86.6(7) . .
O6' W1 O2 62(2) . .
O6 W1 O2 73.6(6) . .
O5 W1 O2 73.2(6) . .
O3 W1 O5' 145.0(18) . .
O4 W1 O5' 109.7(19) . .
O1 W1 O5' 70.1(19) . .
O6' W1 O5' 105(3) . .
O6 W1 O5' 96.8(18) . .
O5 W1 O5' 23.6(17) . .
O2 W1 O5' 60.7(18) . .
O7 W2 O6' 114(2) . .
O7 W2 O8 103.7(7) . .
O6' W2 O8 72(2) . .
O7 W2 O6 99.7(8) . .
O6' W2 O6 25(2) . .
O8 W2 O6 93.8(7) . .
O7 W2 O10 96.3(8) . .
O6' W2 O10 105(2) . .
O8 W2 O10 159.4(7) . .
O6 W2 O10 87.5(8) . .
O7 W2 O9 100.4(7) . .
O6' W2 O9 142(2) . .
O8 W2 O9 87.2(6) . .
O6 W2 O9 159.0(7) . .
O10 W2 O9 84.4(7) . .
O7 W2 O10' 102(2) . .
O6' W2 O10' 122(3) . .
O8 W2 O10' 141(2) . .
O6 W2 O10' 110(2) . .
O10 W2 O10' 25(2) . .
O9 W2 O10' 60(2) . .
O7 W2 O2 168.4(7) . .
O6' W2 O2 63(2) . .
O8 W2 O2 86.2(6) . .
O6 W2 O2 73.3(6) . .
O10 W2 O2 74.5(6) . .
O9 W2 O2 85.9(5) . .
O10' W2 O2 72(2) . .
O5' W3 O11 109(3) . .
O5' W3 O5 29(2) . .
O11 W3 O5 98.9(8) . .
O5' W3 O13 63(3) . .
O11 W3 O13 100.9(7) . .
O5 W3 O13 90.7(7) . .
O5' W3 O10 114(3) . .
O11 W3 O10 99.8(7) . .
O5 W3 O10 90.1(8) . .
O13 W3 O10 158.9(7) . .
O5' W3 O12 139(3) . .
O11 W3 O12 103.3(7) . .
O5 W3 O12 157.8(6) . .
O13 W3 O12 86.7(6) . .
O10 W3 O12 84.6(7) . .
O5' W3 O10' 128(3) . .
O11 W3 O10' 107.4(19) . .
O5 W3 O10' 110(2) . .
O13 W3 O10' 141(2) . .
O10 W3 O10' 23.7(19) . .
O12 W3 O10' 61(2) . .
O5' W3 O2 67(2) . .
O11 W3 O2 170.2(7) . .
O5 W3 O2 73.4(6) . .
O13 W3 O2 85.6(6) . .
O10 W3 O2 74.5(6) . .
O12 W3 O2 84.3(5) . .
O10' W3 O2 70.6(19) . .
O15 W4 O17 103.2(8) . .
O15 W4 O16 101.2(7) . .
O17 W4 O16 93.6(6) . .
O15 W4 O13 100.2(7) . .
O17 W4 O13 86.6(7) . .
O16 W4 O13 157.9(6) . .
O15 W4 O18 100.4(8) . .
O17 W4 O18 155.9(7) . .
O16 W4 O18 86.3(6) . .
O13 W4 O18 84.7(6) . .
O15 W4 O14 174.5(7) . .
O17 W4 O14 81.3(6) . .
O16 W4 O14 75.2(5) . .
O13 W4 O14 83.0(6) . .
O18 W4 O14 75.3(6) . .
O19 W5 O12 103.9(7) . .
O19 W5 O21 100.5(8) . .
O12 W5 O21 89.4(6) . .
O19 W5 O18 95.5(7) . .
O12 W5 O18 87.6(6) . .
O21 W5 O18 164.0(7) . .
O19 W5 O20 99.7(7) . .
O12 W5 O20 156.1(7) . .
O21 W5 O20 89.9(7) . .
O18 W5 O20 86.5(7) . .
O19 W5 O14 169.5(7) . .
O12 W5 O14 82.8(6) . .
O21 W5 O14 87.6(6) . .
O18 W5 O14 76.5(6) . .
O20 W5 O14 73.3(6) . .
O22 W6 O9 101.8(7) . .
O22 W6 O25 100.6(7) . .
O9 W6 O25 85.8(6) . .
O22 W6 O21 98.9(7) . .
O9 W6 O21 89.4(6) . .
O25 W6 O21 160.5(7) . .
O22 W6 O24 100.2(7) . .
O9 W6 O24 157.9(6) . .
O25 W6 O24 87.8(7) . .
O21 W6 O24 89.4(6) . .
O22 W6 O23 172.8(7) . .
O9 W6 O23 84.4(6) . .
O25 W6 O23 76.0(6) . .
O21 W6 O23 84.7(6) . .
O24 W6 O23 73.5(6) . .
O26 W7 O28 105.0(7) . .
O26 W7 O27 100.8(8) . .
O28 W7 O27 95.2(6) . .
O26 W7 O8 99.6(7) . .
O28 W7 O8 87.9(6) . .
O27 W7 O8 157.7(6) . .
O26 W7 O25 98.3(7) . .
O28 W7 O25 155.7(6) . .
O27 W7 O25 87.0(6) . .
O8 W7 O25 81.4(6) . .
O26 W7 O23 170.8(7) . .
O28 W7 O23 83.1(6) . .
O27 W7 O23 73.7(6) . .
O8 W7 O23 84.8(6) . .
O25 W7 O23 74.3(6) . .
O29 W8 O31 102.8(7) . .
O29 W8 O30 101.3(7) . .
O31 W8 O30 91.0(7) . .
O29 W8 O27 97.2(7) . .
O31 W8 O27 88.4(7) . .
O30 W8 O27 161.1(6) . .
O29 W8 O24 96.3(7) . .
O31 W8 O24 160.8(6) . .
O30 W8 O24 86.5(6) . .
O27 W8 O24 87.8(6) . .
O29 W8 O23 167.2(7) . .
O31 W8 O23 87.1(6) . .
O30 W8 O23 86.4(6) . .
O27 W8 O23 74.7(5) . .
O24 W8 O23 73.8(5) . .
O32 W9 O33 103.2(8) . .
O32 W9 O30 100.5(7) . .
O33 W9 O30 88.2(7) . .
O32 W9 O20 97.3(7) . .
O33 W9 O20 158.9(7) . .
O30 W9 O20 83.4(7) . .
O32 W9 O16 100.1(7) . .
O33 W9 O16 92.1(6) . .
O30 W9 O16 158.8(6) . .
O20 W9 O16 89.0(6) . .
O32 W9 O14 167.9(7) . .
O33 W9 O14 87.6(6) . .
O30 W9 O14 84.9(6) . .
O20 W9 O14 72.4(6) . .
O16 W9 O14 74.0(5) . .
O28 Fe1 O3 91.0(7) . .
O28 Fe1 O1 93.0(7) . 2_666
O3 Fe1 O1 91.4(7) . 2_666
O28 Fe1 O17 172.7(6) . 2_666
O3 Fe1 O17 93.4(7) . 2_666
O1 Fe1 O17 92.7(7) 2_666 2_666
O28 Fe1 O2W 86.7(8) . .
O3 Fe1 O2W 176.5(8) . .
O1 Fe1 O2W 86.2(8) 2_666 .
O17 Fe1 O2W 89.2(8) 2_666 .
O28 Fe1 O1W 89.7(6) . .
O3 Fe1 O1W 92.5(7) . .
O1 Fe1 O1W 175.3(8) 2_666 .
O17 Fe1 O1W 84.4(7) 2_666 .
O2W Fe1 O1W 90.0(7) . .
W1 O1 Fe1 176.2(11) . 2_666
Sb1 O2 W1 110.6(6) . .
Sb1 O2 W3 127.9(7) . .
W1 O2 W3 95.1(5) . .
Sb1 O2 W2 129.1(7) . .
W1 O2 W2 94.7(5) . .
W3 O2 W2 90.9(5) . .
W1 O3 Fe1 168.8(10) . .
W1 O4 Fe2 163.5(9) . 2_666
O5' O5 W3 57(5) . .
O5' O5 W1 92(5) . .
W3 O5 W1 118.2(8) . .
O5 O5' W3 95(5) . .
O5 O5' W1 65(4) . .
W3 O5' W1 122(4) . .
O6' O6 W2 66(6) . .
O6' O6 W1 74(5) . .
W2 O6 W1 118.1(9) . .
O6 O6' W2 90(6) . .
O6 O6' W1 83(6) . .
W2 O6' W1 131(4) . .
W2 O8 W7 145.8(8) . .
W6 O9 W2 144.3(8) . .
O10' O10 W2 81(5) . .
O10' O10 W3 89(5) . .
W2 O10 W3 120.0(9) . .
O10 O10' W2 74(5) . .
O10 O10' W3 68(5) . .
W2 O10' W3 111(3) . .
W5 O12 W3 145.7(8) . .
W3 O13 W4 145.3(9) . .
Sb1 O14 W4 116.4(7) . .
Sb1 O14 W5 138.0(7) . .
W4 O14 W5 92.1(5) . .
Sb1 O14 W9 113.6(6) . .
W4 O14 W9 92.5(5) . .
W5 O14 W9 93.9(5) . .
W4 O16 W9 118.3(7) . .
W4 O17 Fe1 141.8(8) . 2_666
W5 O18 W4 115.7(7) . .
W5 O19 Nd1 148.7(8) . .
W5 O20 W9 120.3(8) . .
W5 O21 W6 154.2(8) . .
Sb1 O23 W8 114.0(6) . .
Sb1 O23 W6 138.3(7) . .
W8 O23 W6 95.6(6) . .
Sb1 O23 W7 113.7(7) . .
W8 O23 W7 93.9(5) . .
W6 O23 W7 91.6(5) . .
W6 O24 W8 117.1(7) . .
W6 O25 W7 117.9(8) . .
W7 O27 W8 117.7(7) . .
W7 O28 Fe1 142.9(8) . .
W8 O30 W9 146.6(8) . .
W8 O31 Fe2 133.4(9) . .
W9 O33 Fe2 138.9(8) . .
O11W Nd1 O9W 131.3(14) . .
O11W Nd1 O12W 75.6(13) . .
O9W Nd1 O12W 72.8(13) . .
O11W Nd1 O7W 139.1(14) . .
O9W Nd1 O7W 68.4(14) . .
O12W Nd1 O7W 140.2(14) . .
O11W Nd1 O6W 132.6(10) . .
O9W Nd1 O6W 72.4(11) . .
O12W Nd1 O6W 75.8(10) . .
O7W Nd1 O6W 84.4(12) . .
O11W Nd1 O10W 66.9(14) . .
O9W Nd1 O10W 69.2(14) . .
O12W Nd1 O10W 73.5(13) . .
O7W Nd1 O10W 100.0(15) . .
O6W Nd1 O10W 136.3(13) . .
O11W Nd1 O5W 109.5(12) . .
O9W Nd1 O5W 118.7(13) . .
O12W Nd1 O5W 139.3(11) . .
O7W Nd1 O5W 59.8(13) . .
O6W Nd1 O5W 72.0(11) . .
O10W Nd1 O5W 146.7(13) . .
O11W Nd1 O8W 78.4(12) . .
O9W Nd1 O8W 99.8(11) . .
O12W Nd1 O8W 135.5(11) . .
O7W Nd1 O8W 61.7(13) . .
O6W Nd1 O8W 145.2(10) . .
O10W Nd1 O8W 63.2(13) . .
O5W Nd1 O8W 83.5(11) . .
O11W Nd1 O19 68.0(10) . .
O9W Nd1 O19 135.2(9) . .
O12W Nd1 O19 76.4(9) . .
O7W Nd1 O19 127.8(11) . .
O6W Nd1 O19 69.0(6) . .
O10W Nd1 O19 130.4(11) . .
O5W Nd1 O19 69.3(8) . .
O8W Nd1 O19 125.0(9) . .
O33 Fe2 O31 88.1(7) . .
O33 Fe2 O4 98.8(7) . 2_666
O31 Fe2 O4 96.1(7) . 2_666
O33 Fe2 O34 90.2(7) . .
O31 Fe2 O34 91.2(7) . .
O4 Fe2 O34 168.6(7) 2_666 .
O33 Fe2 O4W 172.9(8) . .
O31 Fe2 O4W 89.5(8) . .
O4 Fe2 O4W 88.1(8) 2_666 .
O34 Fe2 O4W 83.2(8) . .
O33 Fe2 O3W 92.2(8) . .
O31 Fe2 O3W 178.2(8) . .
O4 Fe2 O3W 85.6(8) 2_666 .
O34 Fe2 O3W 87.0(8) . .
O4W Fe2 O3W 89.9(9) . .
C1 O34 Fe2 143(3) . .
C1 O35 H35A 109.5 . .
C3 O36 H36A 109.5 . .
C2 N1 H1A 120.0 . .
C2 N1 H1B 120.0 . .
H1A N1 H1B 120.0 . .
O34 C1 O35 130(5) . .
O34 C1 C2 119(4) . .
O35 C1 C2 110(4) . .
O34 C1 O24W 91(4) . 2_666
O35 C1 O24W 80(4) . 2_666
C2 C1 O24W 107(4) . 2_666
C3 C2 N1 121(4) . .
C3 C2 C1 107(4) . .
N1 C2 C1 104(4) . .
C3 C2 H2A 108.0 . .
N1 C2 H2A 108.0 . .
C1 C2 H2A 108.0 . .
O36 C3 C2 110(4) . .
O36 C3 C4 105(3) . .
C2 C3 C4 108(4) . .
O36 C3 H3A 111.4 . .
C2 C3 H3A 111.4 . .
C4 C3 H3A 111.4 . .
C3 C4 H4A 109.5 . .
C3 C4 H4D 109.5 . .
H4A C4 H4D 109.5 . .
C3 C4 H4B 109.5 . .
H4A C4 H4B 109.5 . .
H4D C4 H4B 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sb1 O14 1.960(14) .
Sb1 O2 1.987(13) .
Sb1 O23 1.998(15) .
W1 O3 1.769(17) .
W1 O4 1.781(16) .
W1 O1 1.793(16) .
W1 O6' 1.97(7) .
W1 O6 2.032(18) .
W1 O5 2.052(17) .
W1 O2 2.233(15) .
W1 O5' 2.26(7) .
W2 O7 1.711(15) .
W2 O6' 1.73(7) .
W2 O8 1.890(15) .
W2 O6 1.898(19) .
W2 O10 1.932(17) .
W2 O9 1.974(14) .
W2 O10' 1.98(7) .
W2 O2 2.349(14) .
W3 O5' 1.58(7) .
W3 O11 1.726(16) .
W3 O5 1.888(18) .
W3 O13 1.903(15) .
W3 O10 1.933(17) .
W3 O12 1.987(14) .
W3 O10' 2.09(7) .
W3 O2 2.349(14) .
W4 O15 1.731(15) .
W4 O17 1.793(16) .
W4 O16 1.921(14) .
W4 O13 1.973(15) .
W4 O18 1.980(16) .
W4 O14 2.291(14) .
W5 O19 1.692(18) .
W5 O12 1.860(14) .
W5 O21 1.887(15) .
W5 O18 1.918(16) .
W5 O20 1.933(15) .
W5 O14 2.292(14) .
W6 O22 1.724(16) .
W6 O9 1.885(14) .
W6 O25 1.895(15) .
W6 O21 1.923(15) .
W6 O24 1.928(14) .
W6 O23 2.311(14) .
W7 O26 1.698(19) .
W7 O28 1.823(14) .
W7 O27 1.911(15) .
W7 O8 1.970(14) .
W7 O25 1.978(15) .
W7 O23 2.319(14) .
W8 O29 1.733(15) .
W8 O31 1.836(18) .
W8 O30 1.917(16) .
W8 O27 1.973(15) .
W8 O24 2.015(15) .
W8 O23 2.230(14) .
W9 O32 1.720(16) .
W9 O33 1.806(17) .
W9 O30 1.949(16) .
W9 O20 1.951(16) .
W9 O16 1.955(14) .
W9 O14 2.317(14) .
Fe1 O28 1.941(14) .
Fe1 O3 1.969(17) .
Fe1 O1 1.970(17) 2_666
Fe1 O17 1.978(16) 2_666
Fe1 O2W 2.093(19) .
Fe1 O1W 2.099(15) .
O5W Nd1 2.51(3) .
O6W Nd1 2.49(2) .
O7W Nd1 2.48(4) .
O8W Nd1 2.52(3) .
O9W Nd1 2.45(3) .
O10W Nd1 2.51(5) .
O11W Nd1 2.44(3) .
O12W Nd1 2.46(3) .
O23W O22W 1.30(10) 2_666
O22W O23W 1.30(10) 2_666
O24W C1 1.90(7) 2_666
O1 Fe1 1.970(17) 2_666
O4 Fe2 1.978(17) 2_666
O5 O5' 0.91(7) .
O6 O6' 0.79(7) .
O10 O10' 0.84(7) .
O17 Fe1 1.978(16) 2_666
O19 Nd1 2.562(18) .
O31 Fe2 1.970(17) .
O33 Fe2 1.943(17) .
Fe2 O4 1.978(17) 2_666
Fe2 O34 2.035(17) .
Fe2 O4W 2.05(2) .
Fe2 O3W 2.077(18) .
O34 C1 1.12(5) .
O35 C1 1.22(6) .
O35 H35A 0.8200 .
O36 C3 1.45(5) .
O36 H36A 0.8200 .
N1 C2 1.479(10) .
N1 H1A 0.8600 .
N1 H1B 0.8600 .
C1 C2 1.65(7) .
C1 O24W 1.90(7) 2_666
C2 C3 1.46(6) .
C2 H2A 0.9800 .
C3 C4 1.70(7) .
C3 H3A 0.9800 .
C4 H4A 0.9600 .
C4 H4D 0.9600 .
C4 H4B 0.9600 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O35 H35A O4W 0.82 2.43 3.10(4) 140.0 .
O35 H35A O25W 0.82 2.52 3.21(5) 142.0 2_656
O36 H36A O24W 0.82 1.74 2.51(6) 156.0 2_666
O36 H36A O12W 0.82 2.28 2.77(5) 118.5 2_655
N1 H1A O22W 0.86 2.40 3.25(11) 167.6 2_655
N1 H1B O30 0.86 2.39 3.13(5) 143.7 .
N1 H1B O29 0.86 2.43 3.11(5) 136.3 .
